Research Inventy: International Journal Of Engineering And ScienceVol.2, Issue 11 (April 2013), Pp 01-05Issn(e): 2278-4721, Issn(p):2319-6483, Www.Researchinventy.Com1Effect of Hardness and Microstructure on En 353 Steel by HeatTreatment1P. Tamil Arasu, 1R. Dhanasekaran, 2P. Senthil Kumar, 3N. Srinivasan1(Department of Mechanical Engineering, K.S.Rangasamy College of Technology, Tamil Nadu, India.1(Department of Mechanical Engineering, K.S.Rangasamy College of Technology, Tamil Nadu, India.2(Department of Mechanical Engineering, K.S.R College of Engineering, Tamil Nadu, India3(Department of Mechanical Engineering, Knowledge Institute of Technology, Tamil Nadu, India.,Abstract : En 353 steel is an easily available and cheap material that is acceptable for heavy duty applications.Heat treatment on En 353 steel is improved the ductility, toughness, strength, hardness and relive internal stressin the material. X-ray diffraction (XRD) method is used to analyze the composition and the phase of the alloymaterial. The experimental results of hardness and microstructure are done to get idea about heat treated En353 steel. It is found that the hardness of the En 353 steel is improved after the heat treatment and themicrostructure is changed from ferrite to martensite.Keywords -En 353 steel, Heat treatment, Hardness, Microstructure.I. INTRODUCTIONEn 353 steel has carbon content of 0.17% and the most common form of steel as it’s provides materialproperties that are acceptable for many automobile applications such as heavy duty gear, shaft, pinion, camshafts, gudgeon pins [1,8]. It is neither externally brittle nor ductile due to its lower carbon content and lowerhardness. As the carbon content increases, the metal becomes harder and stronger.The process of heat treatment is carried out first by heating the metal and then cooling it in water or oilor air. The purpose of heat treatment is, to enhances the transformation of austenite to martensite i.e. (softmaterial to hard material), to change the grain size, to modify the structure of the material and relive the stressset up in the material. It is a one-time permanent treatment process and it is change the entire cross section of thematerial [5, 7]. The martensitic phase transformation is usually used to increase the hardness of the steels.The various heat treatment processes are annealing, normalizing, hardening, quenching and tempering.According to this work basically focus on carburizing; it is a process of improving carbon on case.These are done by exposing the part to carbon rich atmosphere at the high temperature (close to melting point)and allow diffusion to transfer the carbon atoms into the steel. So, these work concentrations go through packcarburizing which can easily do in experimental setup. The carburizing process does not harden the steel it onlyincreases the carbon content. In heat treatments, both chemical composition and microstructure properties of acase can be changed .The aim of this paper is to examine the hardness, XRD and effect of microstructure of before and afterheat treatment on En 353 steel. In heat treatment, the machined specimens are loaded in the chamber at below800°C. Carburizing takes places at 920°C for 120 minutes then it is cooled by air and relaxing time is 75minutes. The purpose of the relaxing time is to arrest the in and out of the carbon and it is followed by oilquenching at 820°C for 30 minutes, oil temperature is below 80°C then by tempering at 250°C for 90 minutes.In general, the untemper material structure has the high hardness and also more brittle. Hence the temperingprocess should be done to reduce the brittleness, to relieve the internal stress and to increase the toughness andductility of the material.Nomenclature :AHT - After Heat TreatmentBHT - Before Heat TreatmentCHT - Conventional Heat TreatmentHV - Vickers Hardness test
Effect Of Hardness And Microstructure…2II. METHODOLOGYAfter heat treatment, the specimens for structure investigations are conventionally prepared and etchedusing nital. The Leica DM 2500 M microscope is used to the observations of obtained structures before and afterthe heat treatment. The specimen with a diameter of 10 mm and a length of 50 mm are subjected to the Hardnesstest using the MH6 machine. X-Ray Diffractometer is one of the most powerful techniques for materialstructural analysis. Bruker AXS D8 Advance XRD machine is to analysis the crystallite size, strain anddislocation density.III. RESULTS AND DISCUSSION3.1 Chemical AnalysisIn order to ensure the material of the specimen is done with help of the optical emission spectroscope(OES). The result is obtain from the chemical analysis, carbon - 0.171 %, silicon - 0.3 %, manganese - 0.56 %,phosphorus - 0.012 %, sulphur - 0.13 %, Chromium – 0.953 %, Nickel - 0.989 %, molybdenum - 0.16 % andremaining percentage is iron respectively. A sample of ϕ 30 × 10 mm is polished using 60 grit papers and twosparks is introduced on the surface to find the chemical composition of the material. After ensuring the chemicalcomposition, the raw material is machined according to the dimension for various tests .3.2 HardnessVickers hardness measurement is done on the specimen as per the IS 1501-2002 procedures by usingVickers hardness tester (MH6). Hardness measurement is made with 200 g loads, dwell time of 10 seconds anddiamond indenter is used for test. The impression is done on the circular faces at the centre of the specimen. Thehardness values are taken corresponding to the diagonal length of the indentation. Two samples (i.e. BHT andAHT) and five readings are taken from the each sample from case to core. The average value is calculated fromfive readings. The hardness values of BHT (case and core) samples are, 193.7 and 201.8 HV respectively. Thehardness values of AHT (case and core) samples are 684.5 and 387.8 HV respectively. It is clearly noticed thatthe base material (BHT) has the low hardness. The AHT specimen has high hardness when compared to theBHT sample as shown in Fig. 1.Figure 1 Micro hardness of the specimen3.3 MicrostructureThe change of microstructure in the material due to conventional heat treatment (CHT) is the mainreason for the improved mechanical properties. Hence the microstructure examination is carried out to find thestructure of BHT and AHT. The samples are polished using SiC emery paper of grit 280 and velvet cloth usingwhite kerosene as coolant. These samples are etched with nital and dried in air. Finally, microstructureexamination is carried out using optical microscope.The effectiveness of the heat treatment process in refining and homogenizing the structure for En 353steel is shown in Fig. 2 to Fig. 7. Fig. 2 to Fig. 4 show the microstructure of BHT is ferrite and spheroidizedpearlite with at the grain boundaries distributed throughout the structure and Fig. 5 to Fig. 7 show themicrostructure of AHT is fine tempered martensite, retained austenite and traces of ferrite distributed throughoutthe structure.
Effect Of Hardness And Microstructure…3Figure 2 the microstructure of BHT (100x)Figure 3 the microstructure of BHT (200x)Figure 4 the microstructure of BHT (500x)Figure 5 the case microstructure of AHT (100x)Figure 6 the core microstructure of AHT (200x)Figure 7 the core microstructure of AHT (500x)
Effect Of Hardness And Microstructure…43.4 XRD AnalysisX-Ray Diffractometer is one of the most powerful techniques for material structural analysis. BrukerAXS D8 Advance X-Ray diffractometer fit with vertical goniometers, low and high temperature attachment.The angle range is 360°, the maximum usable angular is 3° to 135° and wavelength is 1.5406 Å. X-raydiffraction analysis is carried out under the following condition: Cu radiation, 40 KV voltage, 35 mA currentand maximum angular speed 30°/s. When the x-ray is passed into the substrate and it is reflected back to thedetector the angle made by the reflected ray to the substrate is denoted as . The value of is increased bychanging the position of specimen by keeping the as reference β, D, ε, ρ are calculated. The different valuesare obtained by the varying value for certain range.The structural characteristics of En 353 steel material after heat treatment are analyzed by x-raydiffraction analysis. Fig. 8 shows the X-ray diffraction of En 353 steel specimen after heat treatmentrespectively. The estimated crystallite size, strain and dislocation density are calculated from 2θ which lights thepresent of polycrystalline nature of the material. The calculated structural parameters are presented in the Table1.S5-Steel after Heat TreatmentOperations: Smooth 0.200 | Smooth 0.152 | Background 0.813,0.000 | ImportFile: SAIFXR130125B-05(S5-Steel after Heat Treatment).raw - Step: 0.020 ° - Step time: 64. s - WL1: 1.5406 - kA2 Ratio: 0.5 - Generator kV: 40 kV - Generator mA: 35 mA - TyLin(Counts)01002003004005006007008002-Theta - Scale10 20 30 40 50 60 70 80Figure 8 X-ray diffraction peaks of AHTTable 1 X-ray diffraction test results of AHT sampleCos θ Sin θ d-Spacing FWHM βWavelength,λCrystallinesize, DStrain, εDislocationdensity, ρ0.966 0.2585 2.9797 0.244 0.004256 1.54047905 337.189630 0.0010279 8.79532E-060.952 0.3034 2.5385 0.264 0.004605 1.5403436 315.934678 0.0010969 1.00186E-050.879 0.4761 1.6178 0.326 0.005686 1.54045964 277.256040 0.0012501 1.30088E-050.855 0.5182 1.4863 0.318 0.005547 1.54035986 292.221892 0.0011860 1.17105E-05The wave length is calculated by usingλ = 2d sinθ (1)The growth along the peak can be determined by calculating the crystallite size for the peak using (2) Scherrerformula.(2)The full width at half maximum (β) is calculated by using (3) equation.β = FWHM× (3)Strain and dislocation densityThe strain (ε) and the dislocation density (ρ) are calculated from the Williamson-Hall (4) and (5) equation= + (4)ρ = (5)Where, geometrical factor, 0.9 and,λ - The wavelength of X-ray (1.54060 Å),
Effect Of Hardness And Microstructure…5θ - The Bragg diffraction angle in radian andβ - The full width at half maximum of most intense peak.FWHM - Full Width and Half MaximumD - Average crystallite sizeTo ensure a high-quality product, diagrams and lettering MUST be either computer-drafted or drawn using Indiaink. Figure captions appear below the figure, are flush left, and are in lower case letters. When referring to afigure in the body of the text, the abbreviation "Fig." is used. Figures should be numbered in the order theyappear in the text. Table captions appear centered above the table in upper and lower case letters. Whenreferring to a table in the text, no abbreviation is used and "Table" is capitalized.IV. CONCLUSIONBefore and after the heat treatment process the mechanical properties of the En 353 steel are examined.The results obtain under the experimental conditions of this work the following conclusion are drawn. High hardness is obtained in carburizing 120 minutes at 920°C for En 353 steel. Micro hardness values of AHT are found to be higher than BHT. The specimen is having greater hardness on case sample than the core sample. Pictorial view of case/core microstructure indicates that the heat treated specimen is martensite. Thus life of material can be enhanced by the conventional heat treatment process.REFERENCES. A. Bensely, S. Stephen Jayakumar, D. Mohan Lal, G. Nagarajan , and A. Rajadurai, “Failure investigation of crown wheel andpinion”, Engineering Failure Analysis, 13, 2006, 1285–1292.. A. Bahrami, S.H. MousaviAnijdan, M. A. Golozar, M. Shamanian, and N. Varahram, “Effects of conventional heat treatment onwear resistance of AISI H13 tool steel”, Wear, 258, 2005, 846-851.. R. Dhanasekaran, P. Senthil Kumar, and K. Santhi, “Crack failure of planetary gearbox sun gear”, International Journal ofRecent Trends in Engineering and Technology, 3, 2010, 12-14.. M. Ueda, K. Uchino, and A. Kobayashi, “Effects of carbon on wear property in pearlitic steel”, wear, 253, 2002, 107-113.. Narasak Sunwang, Panyamat Wangyao, Yuttanat Boonyongmaneerat, “The effect of heat treatments on hardness and wearresistance in Ni-W alloy coatings”, Surface & Coating Technology, 206, 2011, 1096-1101.. EnverAtık, UmutYunker, and CevdetMerıc, “The effects of conventional heat treatment and boronizing on abrasive wear andcorrosion of SAE 1010, SAE 1040, D2 and 304 steels”, Tribology International, 36, 2003, 155-161.. A. Bensely, A. Prabhakaran, D. Mohan Lal and G. Nagarajan, “Enhancing the wear resistance of case carburized steel (En 353)by cryogenic treatment”, Cryogenics, 2006, 45, 747-754.. H. Khorsand, S.M. Habibi, h.Yoozbashizadea, K. Janghorbon, S.M.S. Reihani, H. Rahmani Seraji, and M.ashtari “The role ofheat treatment on wear behavior of powder metallurgy low alloy steels”, Material and Design, 23, 2002, 667-670.